**HAL Id: hal-00445718**

**https://hal.archives-ouvertes.fr/hal-00445718**

Submitted on 11 Jan 2010
**HAL is a multi-disciplinary open access**

archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Effect of a magnetic field on the two-phonon Raman**

**scattering in graphene**

### Clément Faugeras, Piotr Kossacki, D. M. Basko, Mario Amado, Mike

### Sprinkle, Claire Berger, Walter A. de Heer, Marek Potemski

**To cite this version:**

Clément Faugeras, Piotr Kossacki, D. M. Basko, Mario Amado, Mike Sprinkle, et al.. Effect of a magnetic field on the two-phonon Raman scattering in graphene. Physical Review B: Condensed Matter and Materials Physics (1998-2015), American Physical Society, 2010, 81 (15), pp.155436. �10.1103/PhysRevB.81.155436�. �hal-00445718�

### Effect of a magnetic field on the two-phonon Raman scattering in

### graphene

C. Faugeras,1 _{P. Kossacki,}1, 2 _{D. M. Basko,}3 _{M. Amado,}1, 4 _{M.}

Sprinkle,5 _{C. Berger,}5, 6 _{W.A. de Heer,}5 _{and M. Potemski}1
1_{LNCMI-CNRS, BP 166, 38042 Grenoble, France}

2_{Institute of Experimental Physics, University of Warsaw, Poland}
3_{Laboratoire de Physique et Mod´}_{elisation des Milieux Condens´}_{es,}

Universit´e Joseph Fourier and CNRS, 25 rue des Martyrs, 38042 Grenoble, France

4_{QNS-GISC, Departamento de F´ısica de Materiales,}

Universidad Complutense, E-28040 Madrid, Spain

5_{School of Physics, Georgia Institute of Technology, Atlanta, Georgia 30332, USA}
6_{CNRS-Institut N´}_{eel, BP 166, 38042 Grenoble Cedex 9, France.}

### Abstract

We have studied, both experimentally and theoretically, the change of the so-called 2D band of
the Raman scattering spectrum of graphene (the two-phonon peak near 2700 cm−1_{) in an external}

magnetic field applied perpendicular to the graphene crystal plane at liquid helium temperature. A shift to lower frequency and broadening of this band is observed as the magnetic field is increased from 0 to 33 T. At fields up to 5–10 T the changes are quadratic in the field while they become linear at higher magnetic fields. This effect is explained by the curving of the quasiclassical trajectories of the photo-excited electrons and holes in the magnetic field, which enables us (i) to extract the electron inelastic scattering rate, and (ii) to conclude that electronic scattering accounts for about half of the measured width of the 2D peak.

PACS numbers: 63.22.+m, 63.20.Kr, 78.30.Na, 78.67.-n

I. INTRODUCTION

Graphene, a two-dimensional plane of carbon atoms arranged in a honeycomb lattice,
has stimulated many experimental and theoretical efforts to study and understand its exotic
electronic and optical properties1_{. Graphene can be produced by mechanical exfoliation}

of bulk graphite2_{, by the decomposition of a SiC substrate at high temperatures,}3 _{or by}

epitaxial growth on different metal surfaces4_{. Graphene on SiC is well adapted for }

opti-cal measurements as samples are of macroscopic size and lie on a substrate which can be insulating, and hence, transparent in a wide, from far-infrared to visible spectral range.

Raman scattering is a key element to graphene studies as it is a reliable and
non-destructive technique to establish the monolayer character of a graphene specimen5,6 _{or}

the negligeable interlayer coupling in multilayer epitaxial graphene (MEG) samples7. This
relies on the analysis of the shape of the observed 2D band feature (the two-phonon peak
around 2700 cm−1_{, also referred as D}∗ _{or G}′_{) which is the second-order overtone of the}

D band. While defects (in a general meaning – impurities, interface roughness, etc.) are
needed for the D band to be observed, the 2D band is always seen and it even appears
as the most pronounced feature in the Raman scattering spectrum of graphene. Because
of the doubly-resonant nature of the D band8,9 _{and the fully-resonant nature of the 2D}

band,10,11 _{they both show a dispersive behavior with the excitation energy, what allowed to}

tracing the phonon band structure of different carbon allotropes12,13_{. In this paper, we show}

that a strong magnetic field applied perpendicular to the plane of a graphene crystal signif-icantly affects the 2D band feature. Increasing the magnetic field up to 33 T, we observe a simultaneous red shift of the 2D band energy and a strong broadening of the peak.

In the following, we show that the evolution of the 2D band in magnetic field can be understood and modeled quantitatively as a pure orbital effect of the magnetic field on the intermediate states of the Raman process, i. e., electrons and holes. The field induces circular orbits to the photo-generated electron-hole pairs, and this modifies the momenta of the optical phonons emitted during the Raman scattering process. This leads to a red shift and to a broadening of the 2D band feature as the magnetic field is increased, an effect that we observe experimentally and describe theoretically below. We note that this effect is not specific to a graphene monolayer as the two essential ingredients are the fully-resonant nature of the 2D peak, and the free motion of electrons in the plane. Thus, it should also

be characteristic for the multilayer graphene and graphite.

II. SAMPLES AND EXPERIMENT

Raman scattering measurements were performed in the backscattering geometry at liquid helium temperature and in magnetic fields up to 33 T applied perpendicular to the plane of the graphene crystal. A Ti:Saphire laser tuned at an accurately controlled wavelength of 720 nm (corresponding to the incident photon energy ~ωin = 1.722 eV) was used for

excitation. Optical fibers, both with a core diameter of 200 µm, were used for excitation and for collection. The resulting laser spot on the sample had a diameter of ∼600 µm with a typical power of ∼100 mW.

The samples presented in this study are MEG grown by the thermal decomposition of
the carbon face of a SiC substrate3_{. Despite the fact that these samples contain ∼70 layers,}

simple Dirac-like electronic bands, such as the ones found in exfoliated graphene mono-layers,
persist in these highly graphitized structures because of the particular rotational stacking
exhibited by the adjacent graphitic planes14_{. Dirac Fermions in such MEG structures have}

been evidenced by magneto-transport15_{, by magneto-transmission}16 _{and, more recently, by}

scanning tunnelling spectroscopy17 _{and by magneto-Raman scattering experiments}18_{. Apart}

from the first few interface layers which are highly doped due to the charge transfer from
the SiC substrate15_{, the majority layers, which we probe with Raman scattering, are }

quasi-neutral with densities as low as 5 × 109 _{cm}−2 _{and mobilities as high as 250000 cm}2_{(V · s)}−1_{,}

as deduced from magneto-transmission experiments19_{. MEG samples, and especially the}

highly graphitized specimens, are not homogenous on the scale of our laser spot and contain
some Bernal-stacked inclusions as observed through micro-Raman scattering experiments7_{.}

Typical Raman scattering spectra of the 2D band measured at B = 0, 10, 20 and 30 T are
presented in Fig. 1. At zero field, the 2D band is observed as a slightly asymmetric feature
composed of two Lorentzian contributions. The main contribution to this feature is centered
at 2646 cm−1 _{with a full width at half maximum (FWHM) of 26 cm}−1 _{and the second,}

weaker, contribution is centered at 2675 cm−1 _{with a FWHM of 31 cm}−1_{. As previously}

observed on similar samples7_{, the energy at which the 2D band is observed is increased, for}

a given excitation wavelength, with respect to the energy at which the 2D band is expected for exfoliated graphene flakes. The origin of this effect, probably due to the peculiar type

of stacking of the graphitic planes and the resulting electronic interaction between these
planes, is still a matter of debate20,21_{. The origin of the double component 2D band feature}

observed in our experiment, different than the one observed in bulk graphite, is still not
clear. It could be due to Bernal-stacked inclusions under the large laser spot. We note that
similar line shapes have also been observed in micro-Raman scattering measurements on
epitaxial graphene samples on SiC and were interpreted as revealing graphene domains with
different amount of strain22_{. When a magnetic field is applied perpendicular to the graphene}

crystal plane, both of these two components show a red shift and a broadening. We present
in Fig. 2 the evolution of the Raman shift and of the FWHM of both components of the 2D
band with magnetic field. From B = 0 to 33 T, a shift of ∼ 8 cm−1 _{and an increase of 20%}

of the FWHM is observed.

III. DISCUSSION

From the very beginning, we would like to stress that the observed effect is quite
un-likely to be related to the modification of the spectrum of the emitted phonons (e. g., by
electron-phonon interaction). Indeed, electrochemically top gated graphene structures
al-lowing to tune the Fermi level up to 800 meV (carrier density up to ∼ 4×1013 _{cm}−2_{) have}

been produced recently.23,24 _{Raman scattering experiments in these highly doped }

struc-tures showed that the evolution of the 2D band central frequency with doping is moderate and monotonous, and can be described by a change of the equilibrium lattice parameter without considering any dynamical effects. Modification of the phonon dispersion due to the electron-phonon coupling is noticeable near the K point of the phonon band structure (Kohn anomaly), while the phonons involved in the 2D band are too far from the K point to be affected by the Kohn anomaly. As a result, no effect related to the electron-phonon coupling is observed on the 2D band. This argument remains valid even in magnetic fields used in our experiment. Indeed, the magnetic field mixes wave vectors on the scale of the inverse magnetic length, 1/lB =peB/(~c) ≈ 0.022 ˚A

−1

at B = 33 T. The wave vector of the phonons responsible for the 2D peak, measured from the K point, is q ≈ 0.24 ˚A−1 at 1.7 eV excitation. Thus, q ≫ 1/lB and the Kohn anomaly remains inaccessible for these

phonons even at our highest fields. This is in striking contrast with the main first-order Ra-man feature, the so-called G band due to the doubly degenerate E2g optical phonons at the

### 2400

### 2500

### 2600

### 2700

### 2800

## in

## te

## n

## s

## it

## y

## (

## a

## rb

## .

## u

## n

## it

## s

## )

## Raman shift

### (

## cm-1

### )

### B = 0T

### B = 10T

### B = 20T

### B = 30T

FIG. 1: (Color online) Experimental Raman scattering spectra measured at T = 4.2 K in the 2D band range of energy at different values of the magnetic field (black solid line), two Lorentzian fits (red solid line) and independent components of the Lorentzian fits (black dotted lines). The vertical black dashed line is a guide for the eyes.

### 25

### 30

### 35

### 40

### F

### W

### H

### M

### (

### c

### m

### -1

### )

### 25

### 30

### 35

### 40

### 0

### 10

### 20

### 30

### 2636

### 2638

### 2640

### 2642

### 2644

### 2646

### 2648

### R

### a

### m

### a

### n

### s

### h

### if

### t

(### c

### m

### -1

)### B (T)

### 0

### 10

### 20

### 30

### 2666

### 2668

### 2670

### 2672

### 2674

### 2676

### 2678

### B (T)

## a)

## d)

## b)

## c)

FIG. 2: (Color online) a) FWHM and b) Raman shift of the low-energy component of the 2D band as a function of the magnetic field. c) FWHM and d) Raman shift of the high-energy component of the 2D band as a function of the magnetic field. Solid red lines are calculated with our model (see text).

Γ point of the phonon band structure. These phonons are directly in the region of the Kohn
anomaly, and their frequency and lifetime are noticeably affected even by a moderate gate
voltage.25,26 _{In strong magnetic fields, the G band exhibits a pronounced magneto-phonon}

effect,18 _{as the phonon state is modified by the coupling to electronic inter-Landau-level}

transitions.27,28

In the following, we show that our observations are due to the finite curvature of the
trajectories of the photo-excited electrons and holes in the magnetic field. The main idea
is illustrated in Fig. 3. In the semi-classical real-space picture of the Raman process,29 _{the}

incident photon creates an electron and the hole with opposite momenta at an arbitrary
location within the laser spot. They subsequently propagate along the classical trajectories,
and emit phonons. If they meet at some other location, again with opposite momenta, they
can recombine radiatively producing a scattered photon. In the absence of the magnetic
field, the trajectories are straight lines, so that in order to meet at the same point with
opposite momenta and contribute to the Raman scattering signal, the electron and the hole
must necessarily be scattered backwards during the phonon emission.29_{This fixes the phonon}

momentum ~q (measured from the K or K′ _{point) as q = p + p}′_{, where ~p = ~ω}

in/(2v) and

~_{p}′ _{= ~(ω}_{in}_{− 2ω}_{ph}_{)/(2v) are the electronic momenta (also measured from the Dirac points)}
before and after the phonon emission, ωin is the excitation frequency, ωph is the phonon

frequency, and v is the electronic velocity (the slope of the Dirac cones). A slight spread
in the phonon momentum due to the quantum uncertainty, |q − p − p′_{| ∼ 2γ/v (2γ being}

the electron inelastic scattering rate), gives a contribution to the width of the 2D peak, ∼ 2γ(vph/v), where vph = dωph/dq is the phonon group velocity.29

In a magnetic field, the electron and hole trajectories are no longer straight lines but,
because of the Lorentz force that acts on charged particles in a magnetic field, they
corre-spond to circular cyclotron orbits. As a result, one can see from Fig. 3 that (i) phonons
with smaller momenta, q = p cos ϕ + p′_{cos ϕ}′_{, can be emitted, and (ii) since each phonon}

can be emitted at an arbitrary instant in time, the length of the arc describing the
elec-tron trajectory is random [not exceeding the elecelec-tron mean free path v/(2γ)], and so are
the angles ϕ, ϕ′_{. Tuning the magnetic field is, in this sense, equivalent to changing the}

resonant conditions of the Raman scattering process at a fixed excitation wavelength and allows exploring part of the phonon band structure closer to the K point. Fact (i) results in the overall red shift of the Raman peak, while fact (ii) introduces an additional spread

in q, and contributes significantly to the broadening of the peak as observed through Raman scattering measurements.

To produce the observed effects, the electron and the hole do not have to complete a full
orbit. The probability of this latter event vanishes as e−2πR(2γ/v)_{, where R = p(eB/~c)}−1

is the cyclotron radius. This implies that the separation between the electronic Landau levels, ~ωc = ~v/R, may still be smaller than their broadening 2~γ and, in our experiment,

this is still the case even at B = 30 T. In other words, even magnetic fields far from the
quantization limit can give a noticeable effect. A closely related effect has been discussed
in the context of density-density response of a degenerate electron gas in a non-quantizing
magnetic field30_{.}

To obtain some more quantitative information about the behavior of the 2D peak in
magnetic fields, we calculate the Raman matrix element M(q) for a given phonon wave
vector q in a clean graphene monolayer. It is convenient to perform the calculation in the
coordinate representation, analogously to the calculation for the D peak in the vicinity of
an edge31 _{(details of this calculation are presented in the Appendix). An essential ingredient}

of the calculation is the semiclassical electronic Green’s function for graphene in a magnetic field which was calculated in Ref. 32. Under the assumption ωc ≪ (γ, ωph) ≪ ωin, the result

of the calculation can be represented as:

M(q) ∝ ∞ Z 0 dz√z e−[i(q−2p)+2γ/v]z−i[p/(12R2)]z3 = = 2(iπ)3/2 R

√_{p} _{du}d Ai2(u) − i Ai(u) Bi(u) , (1)
u →
q − 2p − 2iγ
v
R2
p
1/3
. (2)

For vanishing magnetic fields, the cyclotron radius R → ∞ and the relation M(q) ∝ (q −
2p − 2iγ/v)3/2_{, which is Eq. (64) of Ref. 29, is recovered. For finite values of the magnetic}

field, the matrix element is expressed in terms of Airy functions Ai(u) and Bi(u)33_{. Note}

also the similarity with the expression for the polarization operator in Ref. 30.
Since the density of the final phonon states is practically q-independent34_{, |M(ω}

in/v +

Ω/(2vph))|2 describes the Raman scattering intensity as a function of Ω, the Raman shift

measured with respect to the center of the 2D peak at zero field. To illustrate the change of the peak shape in magnetic fields, we present in Fig. 4(a) |M(ωin/v + Ω/2vph)|2 for

**q**

## ϕ

**q**

## ϕ

FIG. 3: (Color online) Schematic of the electron and hole motion during the Raman scattering process. The lightening represents the incident photon which creates the electron-hole pair. The solid arcs denote the propagation of the electron and the hole in the magnetic field. The flash represents the radiative recombination of the electron-hole pair. The dashed arrows denote the emitted phonons.

B = 0, 10, 30 T, considering ~ωin = 1.7 eV, ~v = 7 eV · ˚A (v = 1.06 × 108 cm/s), vph/v =

50 cm−1_{/eV, ~γ = 27 meV. This value for γ is chosen in order to reproduce the observed}

shift of the peak maximum for increasing magnetic fields. However, the resulting FWHM
for the 2D band is about twice smaller than the one observed experimentally at zero field.
Most likely, this indicates the presence of an additional broadening mechanism besides the
electronic scattering. As we cannot determine the nature of this mechanism, we model
it by introducing phenomenologically an additional broadening of the 2D band through a
convolution of |M|2 _{with a Gaussian curve of width σ:}

I2D(Ω) ∝
∞
Z
−∞
dΩ′
√
2πσ e
−(Ω′−Ω)2_{2σ2}
M
ωin
v +
Ω′
2vph
2
. (3)

There is no simple relation between the FWHM of the original |M|2 _{peak}

(8γ(vph/v)

√

22/3_{− 1 at zero field), the FWHM of the broadening Gaussian (2σ}√_{ln 4), and}

the FWHM of the resulting peak. The result of the convolution for σ = 9.5 cm−1 _{is shown}

in Fig. 4(b).

In the following, we assume γ and σ to be independent of the magnetic field. This

-40 -30 -20 -10 0 10 20

### relative Raman shift (cm

-1### )

0 5 10 15 20### Intensity (a.u.)

-40 -30 -20 -10 0 10 20### relative Raman shift (cm

-1### )

0 5 10 15 20### Intensity (a.u.)

### (a)

### (b)

FIG. 4: (a) |M|2 _{as given by Eq. (1) for γ = 27 meV. (b) convolution of |M|}2 _{with a 9.5 cm}−1_{-wide}

Gaussian curve as given by Eq. (3). Solid, dashed, and dotted lines correspond to B = 0, 10, 30 T, respectively. The Raman shift is measured with respect to the center of the peak at zero field.

approximation is reasonable as long as the magnetic field is non-quantizing.35 _{At B = 30 T,}

electrons with energy ǫ = 0.85eV measured from the Dirac point, have a cyclotron frequency ωc = (v2~/ǫ)(eB/~c) of about 27 meV, so the strongest magnetic fields in this experiment

seem to be close to the limits of validity of this approximation. Beyond this regime, Landau quantization of the electronic spectrum should manifest itself as oscillations of the peak intensity due to periodic modifications of the resonance conditions with increasing magnetic field, while in the experiment no such oscillations are observed.

The results of this calculation in terms of Raman shift and of FWHM of the peak, as
described by Eq. (3), are presented as red solid lines in Fig. 2 (a)–(d) for the two components
of the observed 2D band feature. The following parameters were adjusted: (i) the central
frequencies of the two components at zero field, giving the overall vertical offset for the curves
in Fig. 2 (b), (d); (ii) σ = 9.5 cm−1 _{and σ = 11.9 cm}−1 _{were taken for the low-frequency and}

high-frequency components, respectively, in order to reproduce the FWHM at zero field, in combination with (iii) ~γ = 27 meV which determines all four slopes in Fig. 2 (a)–(d). Clearly, without precise knowledge of the origin of the two 2D band components we cannot account for the slight difference in their zero-field widths. Nevertheless, the fact that the calculation reproduces the red shift of the 2D band energy as a function of the magnetic

### 0

### 5

### 10

### 15

### 20

### 25

### 30

### 35

### 0

### 5

### 10

### 15

### 20

### 25

### 30

### In

### te

### g

### ra

### te

### d

### I

### n

### te

### n

### s

### it

### y

### (

### a

### rb

### .

### u

### n

### it

### s

### )

### B (T)

FIG. 5: Integrated intensity of the 2D band low energy component (black dots) and of the 2D band high energy component (open circles) as a function of the magnetic field.

field which is quadratic for fields up to 5–10 T and linear at higher fields, with a single value of γ for both components, shows that the electrons have the same dynamics in the parts of the sample, responsible for the two components.

Besides, the deduced value of ~γ = 27 meV is in good agreement with that deduced
from the doping dependence of the 2D peak intensity in exfoliated graphene36,37 _{(given the}

energy dependence of γ and the fact that the latter measurements were performed at higher
excitation energy, the electron scattering in those samples is somewhat weaker than in ours).
We also note that the found value ~γ = 27 meV is in reasonable agreement with the line
width of electronic transitions in high magnetic fields measured in this range of energy on
similar samples.38 _{This fact is remarkable because those measurements were performed in a}

quantizing magnetic field, and a priori the scattering rate does not have to be the same.35

From Eq. (1) it can be seen that the integral R |M(q)|2_{dq does not depend on the }

mag-netic field. (It is sufficient to integrate over q first, and then over z; the magmag-netic field enters only through R, which drops out.) This means that under the assumption of a constant phonon density of states, the frequency-integrated intensity (the area under the peak) of the 2D band should not depend on the magnetic field. The experimental intensities for the two components are plotted on Fig. 5. Only the integrated intensity of the high-frequency component is field independent, while an overall decrease of ∼ 35% of the integrated inten-sity of the low-frequency component is observed over the range of B between 0 and 33 T. Does it mean that the phonon density of states decreases stronger for the lower-frequency component? Again, without precise knowledge of the exact nature of the two components it is hard to give an explanation for their different behavior.

IV. CONCLUSIONS

In conclusion, we have studied, both experimentally and theoretically, the evolution of the 2D band of MEG structures in intense magnetic fields. We observe a red shift and a broadening of the 2D band as the magnetic field is increased. We have modelled this effect using a semi-classical picture in which the Lorentz force induced by the magnetic field on the photo-created electron-hole pairs, curves the carriers trajectories. This leads to a decrease of the emitted optical phonon momentum and a broadening of the 2D band as observed through Raman scattering spectroscopy. This model enables us to extract the value of the electronic scattering rate. From this we conclude that about half of the 2D band width at zero field is due to electronic scattering while the origin of the other half remains to be clarified. Finally, we note that the observed effect of the magnetic field on the 2D peak is not specific to monolayer graphene; it should be analogous for multilayer graphene and graphite.

Acknowledgments

Part of this work has been supported by EC MTKD-CT-2005-029671, EuromagNetII, PICS-4340, ANR-08-JCJC-0034-01 and ANR-06-NANO-019 projects. P.K. is financially supported by the EU under FP7, contract no. 221515 ‘MOCNA’. M. A. thanks the Cariplo Foundation (project QUANTDEV), MICINN (Project MOSAICO) and JCYL SA052A07 for support.

APPENDIX A: QUASICLASSICAL CALCULATION OF THE TWO-PHONON RAMAN MATRIX ELEMENT IN A UNIFORM MAGNETIC FIELD

1. Classical action for a Dirac particle

The two-phonon Raman matrix element is given by a loop of four electronic Green’s
functions. The latter will be taken in the quasiclassical approximation. The most important
ingredient of the quasiclassical Green’s function is the classical action. Thus, we first discuss
the classical action, then we give the explicit expression for the electronic Green’s function,
and finally, we perform the calculation of the Raman matrix element. In fact, the first two
steps have been already made by Carmier and Ullmo32_{, but we include them here for the}

sake of completeness of the presentation, and to fix the notations.

We start with the classical equation of motion of a charge in the magnetic field B: dp

dt = e

cv× B (A1)

For a Dirac electron with energy ǫ the velocity v(t) = vn(t) and momentum p(t) = (ǫ/v)n(t)
are expressed in terms of a unit vector, |n| = 1. [If instead of electrons with positive
and negative energies one prefers to work with positive-energy electrons and holes, then
p_{(t) = |ǫ/v|n(t), so the action given below should be multiplied by sgn ǫ]. Eq. (A1) can be}
obtained by variation of the action functional

S[r(t)] = Z dtǫ v |˙r| + e cA(r) · ˙r (A2)

keeping the ends r1, r2 of the trajectory fixed. Indeed, upon integration by parts

δS =
Z
dt
−_{v}ǫ _{dt}d ˙xi
|˙r| +
e
c ˙xj
∂Aj
∂xi −
∂Ai
∂xj
δxi
+ p2 · δr2− p1 · δr1, (A3)
13

where indices i, j = x, y, z label the Cartesian components, and the momentum is defined
as
p_{≡} ǫ
v
˙r
|˙r| +
e
cA(r). (A4)

If we now define the function S(r, r′_{) as the action on the classical trajectory, corresponding}

to the motion from r′ _{to r according to Eq. (A1), we obtain ∇S = p at the end of the}

trajectory. Thus, this function satisfies the Hamilton-Jacobi equation
∇S (r, r
′
) −e_{c}A(r)
=
−∇
′_{S(r, r}′
) − e_{c}A(r′)
=
|ǫ|
v . (A5)

Also, ∂S/∂ǫ is equal to the time it takes to go along the trajectory.

In a uniform magnetic field, n is precessing with a constant frequency ω = −(eB/c)(v2_{/ǫ),}

and the trajectories are circles of the radius R = v/|ω|. Two particular points r and r′ _{can}

be connected either by two trajectories corresponding to short and long arcs (plus an integer
number of full rotations), or by no trajectories at all if the distance between the points is
greater than the circle diameter, |r − r′_{| > 2R. Let us assume B to be along the z axis and}

choose the gauge A(r) = (B/2)[ez× r]. The action along the short/long arc is given by

S±(r, r′) =
ǫR
2v [ϑ±(r, r
′_{) + sin ϑ}
±(r, r′)]
− eB_{2c} [r × r′]z, (A6)
ϑ+(r, r′) = 2 arcsin|r − r
′_{|}
2R , (A7)
ϑ−(r, r′) = 2π − 2 arcsin|r − r
′_{|}
2R . (A8)

Here ϑ±(r, r′) is the angular size of the short/long arc. We also introduce ϑ(j)± (r, r′) =

2πj + ϑ±(r, r′). We denote by n± the unit tangent vector to the short/long arc at the point

r (Fig. 6):
n_{±}(r, r′) =
e_{z}_{×} r− r
′
|r − r′_{|}
sinϑ±(r, r
′_{)}
2 sgn ω
+ r− r
′
|r − r′_{|}cos
ϑ±(r, r′)
2 . (A9)

The tangent determines the direction of the kinematic momentum:

∇S±(r, r′) −
e
cA(r) =
ǫ
vn±(r, r
′_{),} _{(A10)}
−∇′_{S}
±(r, r′) −
e
cA(r
′_{) = −}ǫ
v n∓(r, r
′_{).} _{(A11)}
14

**n**

_{−}

**n**

_{+}

**n**

_{−}

**n**

_{+}

### +

### ϑ

*R*

**r’**

**r**

FIG. 6: (Color online) Two classical trajectories connecting the points r, r′_{.}

2. Quasiclassical Green’s function

Now we discuss the Green’s function for the Dirac equation,

h

ǫ + i~γǫsgn ǫ + vΣ ·

i~∇ + e_{c}AiG(r, r′)

=1_{1 δ(r − r}′). (A12)

Here Σ = (Σx, Σy) are the pseudospin matrices in the sublattice space, 11 is the unit matrix,

and γǫ > 0 is the half of the electron or hole inelastic scattering rate, introduced

phenomeno-logically (see Sec. IVC of Ref. 29 for the discussion of its role in Raman scattering). The factor sgn ǫ corresponds to the chronologically ordered Green’s function.

The quasiclassical Green’s function is represented as a sum over all trajectories of the
classical motion from r′ _{to r, i. e., sum over the short and long arcs, “±”, and over the}

number of rotations j = 0, 1, . . .:
G(r, r′) =
∞
X
j=0
h
G(j)+ (r, r′) + G
(j)
− (r, r′)
i
, (A13)
G(j)_{±} (r, r′) = e±iπ/4sgn ǫ
s
|ǫ|/(~v)3
2πR| sin ϑ(j)± (r, r′)|
×
× ψn±(r,r′)ψ
†
−n∓(r,r′)e
−i(eB/2~c)[r×r′_{]}
z
×
× ei[ϑ(j)±(r,r′)+sin ϑ
(j)
±(r,r′)]|ǫ|R/(2~v)×
× e−ϑ(j)±(r,r′)γǫR/v_{.} _{(A14)}

The imaginary part of the argument of the exponential is just the classical action discussed
in the previous subsection. Replacement ǫ → |ǫ| is required by the analytical properties of
the chronologically ordered Green’s function (otherwise it would correspond to the retarded
Green’s function). The damping factor e−γǫϑR/v _{is determined by the total length of the}

corresponding arc ϑR, including 2πjR from j full rotations. The eigenvector ψn of (n ·

Σ)ψn = ψnsgn ǫ, |n| = 1, can be written in terms of the polar angle ϕn of the unit vector n

(we use the basis where Σx, Σy are represented by Pauli matrices),

ψn = 1 √ 2 e−iϕn/2sgn ǫ eiϕn/2 . (A15)

Thus defined, ψn is not a single-valued function: when n is rotated by 2π, ψn acquires

a minus sign. We can fix the sign by requiring that at r → r′_{, ψ}

n+ = −ψ−n− = ψr−r′,

ψn− = ψ−n+ = ψr′−r, and they evolve continuously during the motion along the circle.

We make several further remarks concerning the above expression for G(r, r′_{),}

Eqs. (A13), (A14).

(i) For r → r′ _{G(r, r}′_{; ǫ) reduces to the expression for the quasiclassical Green’s function}

for B = 0,
G0(r − r′; ǫ) = −
eiπ/4
2
11 sgn ǫ + r− r
′
|r − r′_{|}· Σ
×
s
|ǫ|/(~v)3
2π|r − r′_{|}e
(i|ǫ|/~−γǫ)|r−r′|/v_{,}
(A16)
valid at |ǫ||r − r′_{|/(~v) ≫ 1.}
16

(ii) The difference between the exact Green’s function and G(r, r′_{; ǫ) given by}

Eqs. (A13), (A14) is of higher order in ~. This can be checked explicitly by calculating
the gradients:
dϕn±(r,r′) = −
[n∓× dr]z
R sin ϑ±
= [n∓× dr
′_{]}
z
R sin ϑ±
, (A17)
∇ sin ϑ±=
1
R
cos ϑ±
cos(ϑ±/2)
r_{− r}′
|r − r′_{|}, (A18)
∇ψn+ =
1
2iΣzψn+∇ϕn+
= 1
2iΣzψn+
[ez× n−]
R sin ϑ+
, (A19)
(Σ · ∇)ψn+ = −
(n−· Σ)ψn−
2R sin ϑ+
, (A20)
so that at r 6= r′
[ǫ + iγǫsgn ǫ + i~vΣ · ∇]G(j)+ (r, r′; ǫ) =
= − i~v
R cos2_{(ϑ}
+/2)
[n+× Σ]zG(j)+ (r, r′; ǫ). (A21)

It is proportional to the eigenvector corresponding to the energy −ǫ; thus, it can be com-pensated by a correction to the pre-exponential factor which does not vanish when acted upon by ǫ + ivΣ · (∇S − ieA/c), and thus is of the next order in ~:

δG(j)+ (r, r′; ǫ) =
i~v
2ǫR cos2_{(ϑ}
+/2)
[n+× Σ]zG(j)+ (r, r′; ǫ). (A22)
δG(j)+ is smaller than G
(j)

+ by the dimensionless parameter ~v/(ǫR). However, it has a

stronger divergence at |r − r′_{| → 2R; this is the manifestation of the usual breakdown of the}

quasiclassical approximation in the vicinity of the classical turning point.

(iii) To fix the relative phases of G(j)_{+} and G(j)_{−} we choose a given circular trajectory
and consider the evolution of G(r, r′_{; ǫ) as r moves along the circle. Namely, as r passes the}

turning point at |r−r′_{| = 2R, G}(j)

+ (r, r′; ǫ) should transform into G (j)

− (r, r′; ǫ). In the vicinity

of the turning point, |r − r′_{| = 2R(1 + z), z ≪ 1, we have ϑ}

± ≈ π ∓√−2z. Thus, ϑ± can be

viewed as two branches of the same analytical function, and ϑ+ → ϑ− when z makes a circle

around z = 0 in the complex plane. Since ϑ±+ sin ϑ± ≈ π ∓ (−2z)3/2/6, in order to get a

decaying exponential in the classically forbidden region |r − r′_{| > 2R (the positive semiaxis}

of z), the circle must be counterclockwise. Thus,
eiπ/4
q
sin ϑ(j)_{+}
→ e
−iπ/4
q
| sin ϑ(j)− |
, (A23)
17

precisely as in Eq. (A14).

(iv) To match the phases of G(j)− and G (j+1

+ ), we consider r → r′ and require that

G(j)_{−} (r, r′_{; ǫ)+G}(j+1)

+ (r, r′; ǫ) satisfies the homogeneous Dirac equation. Indeed, the δ-function

term is produced by G(0)+ component, see remark (i). At r → r′ the Green’s function

satis-fying the homogeneous Dirac equation can be can be constructed in the B → 0 limit. Let us introduce ¯G0(r − r′; ǫ), the Green’s function with analytical properties opposite to those

of G0:
¯
G0(r − r′; ǫ) =
e−iπ/4
2
−11 sgn ǫ + r− r
′
|r − r′_{|} · Σ
×
s
|ǫ|/(~v)3
2π|r − r′_{|}e
(−i|ǫ|/~+γǫ)|r−r′|/v_{.}
(A24)

It also satisfies Eq. (A12), as seen from the antisymmetry of the Dirac operator with respect to the simultaneous change ǫ → −ǫ, i → −i, γǫ → −γǫ. Thus, G0(r − r′; ǫ) − ¯G0(r − r′; ǫ)

represents the sought solution, corresponding to the flux of particles focusing at the point r′_{.}

Hence, the correspondence is G(j)− (r → r′; ǫ) ∼ − ¯G0(r − r′; ǫ) (converging wave), G(j+1)+ (r →

r′_{; ǫ) ∼ G}0(r − r′; ǫ) (outgoing wave), which produces precisely the combination of signs as

in Eq. (A14).

Remarks (iii) and (iv) can be restated in very simple terms. Upon every half-rotation
sin ϑ changes sign, so the square root produces a factor of eiπ/2_{. In addition, upon a full}

rotation ψn acquires the Berry phase eiπ. Hence, the sum over j in Eqs. (A13), (A14) reduces

to a simple geometric progression,

∞

X

j=0

ejπ(i|ǫ|/~−2γ)R/v = 1

1 − eπ(i|ǫ|/~−2γ)R/v, (A25)

which determines the poles corresponding to πǫR/~v being an integer multiple of 2π, i. e., Bohr-Sommerfeld quantization rule. It gives the exact expression for the Landau levels, |ǫn/v| =p2n|e~B/c|.

3. Two-phonon Raman matrix element

Here we consider the matrix element M(q; ϕin, ϕout) for the transition from the initial

state, corresponding to the incident photon with frequency ωinpolarized at the angle ϕin to

the x axis, and no phonons, to the final state, corresponding to the scatterd photon with frequency ωin−2ωqpolarized at the angle ϕout to the x axis, and two phonons with momenta

q_{, −q and frequencies ω}q (q is measured from the K or K

′ _{point, and for the phonons in}

the two valleys the frequencies ωq(K) = ω
(K′_{)}

−q due to the time-reversal symmetry; we denote

ωq(K) ≡ ωq and omit the valley index). Then, for unpolarized excitation and detection, the

frequency-resolved intensity I(Ω) is given by

I(Ω) ∝
2π
Z
0
dϕin
2π
dϕout
2π
Z
d2_{q}
(2π)2
× |M(q; ϕin, ϕout)|2δ(Ω − 2ωq). (A26)

The matrix element is given by the loop of four Green’s function with electron-photon and
electron-phonon vertices (here we write it in the coordinate representation)29_{:}

M(q; ϕin, ϕout) ∝ Z dǫ 2π Z d2r2d2r1d2r0d2r′1

× Tr {(Σxcos ϕout+ Σysin ϕout)

× G(r2, r1; ǫ + ωin/2 − ωq) × Σze−iqr1G(r1, r0; ǫ + ωin/2) × (Σxcos ϕin+ Σysin ϕin) × G(r0, r′1; ǫ − ωin/2) Σzeiqr ′ 1 × G(r′1, r2; ǫ − ωin/2 + ωq)} . (A27)

We will assume γωin/2R/v ≫ 1 (non-quantizing field), then the probability of a half- or

full rotation is exponentially small, and only the G(0)_{+} contribution to the Green’s functions
remains. The integral over ǫ is dominated by small |ǫ| ∼ γωin/2, so the energy arguments of

the Green’s functions can be assumed to have definite signs. Thus, the imaginary part of the exponent can be written as

S(r2, r1; ωin/2 − ωq+ ǫ) − qr1+ S(r1, r0; ωin/2 + ǫ)

+ S(r0, r′1; ωin/2 − ǫ) + qr′1

+ S(r′_{1}, r2; ωin/2 − ωq+ ǫ), (A28)

where the action S is that given by Eq. (A6), with the “+” subscript omitted and the energy argument explicitly introduced.

The spatial integration is performed in the stationary point approximation. Namely, in the whole 8-dimensional space (r0, r1, r′1, r2) we separate a manifold on which

expres-sion (A28) is stationary. As ∇S is just the classical momentum, this manifold corresponds to joining the classical arcs connecting the pairs of points in order to satisfy momentum conservation at each point r0, r1, r′1, r2. Then the integration over the deviations from this

manifold is performed in the Gaussian approximation, while the integration over the mani-fold itself has to be done more carefully. This procedure is fully analogous to that used in Sec. VIB of Ref. 31 for the edge-assisted Raman scattering.

The integration over ǫ will be performed by expanding the actions to the linear order, e. g. S(r1, r0; ωin/2 + ǫ) → → S(r1, r0; ωin/2) + ∂S(r1, r0; ωin/2 + ǫ) ∂ǫ ǫ=0 ǫ, (A29)

and neglecting the ǫ-dependence of the pre-exponential factors. Then the integration over ǫ
gives a δ-function, δ(t01+ t12− t21′− t_{1}′_{0}), where t_{ij} is the time of travel from the point i to

the point j according to the classical equations of motion. This δ-function simply expresses the fact that the electron and the hole have to travel for the same amount of time before the radiative recombination.

Let us assume the phonon momentum q to be along the y axis. Out of eight spatial integration variables two correspond to translations of the trajectory as a whole. They con-tribute to normalization, but as we are not interested here in the overall prefactor in M(q), they can be discarded. In the remaining 6-dimensional space we introduce three coordinates y1, ϕ, ϕ′ which parametrize the stationary manifold, and three deviations δx1, δR, δR′. The

integration variables are parametrized as (see Fig. 7):

r0 =
R cos ϕ −
q
R2_{− y}2
1, R sin ϕ

+ (δR cos ϕ, δR sin ϕ), (A30)

r1 = (0, y1) + (δx1, 0), (A31)
r′_{1} _{= (0, −y}1) + (−δx1, 0), (A32)
r_{0} =
−R′_{cos ϕ}′_{−}q_{(R}′_{)}2_{− y}2
1, R′sin ϕ′

+ (−δR′cos ϕ′, δR′sin ϕ′), (A33) 20

**p**

**p**

**q**

*R*

*R*

### ϕ

### −ϕ

**r**

_{1}

**r**

**r**

**r**

_{1}

### 0

### 2

### 1

*y*

FIG. 7: (Color online) Classical trajectories determining the stationary manifold.

where R = p/(eB/c), R′ _{= p}′_{/(eB/c), p = ω}

in/2v, p′ = (ωin− ωq)/2v. If we introduce

ϕ1 = arcsin(y1/R), ϕ′1 = arcsin(y1/R′), then momentum conservation reads as

p sin ϕ1 = p′sin ϕ′1, p cos ϕ1+ p′cos ϕ′1 = q . (A34)

This ensures that the expansion of Eq. (A28) in the deviations does not have linear terms. Now we have to expand Eq. (A28) to the second order in δx1, δR, δR′. If we denote

s_{≡} r− r

′

|r − r′_{|}, (A35)

the second derivatives of the action can be written as ∂S ∂xi∂xj = ∂S ∂x′ i∂x′j = = eB 2c −sisjtan ϑ+ 2 + (δij − sisj) cot ϑ+ 2 , (A36) ∂S ∂xi∂x′j = eB 2c × × sisjtan ϑ+ 2 − (δij − sisj) cot ϑ+ 2 − eijz , (A37)

where exyz = −eyxz = 1, exxz = eyyz = 0. As a result, for the quadratic part of the action

∆S we have

∆S = −eB_{2c} sin 2ϕ1(δR − δx1cot ϕ1sin ϕ)

2
sin(ϕ1− ϕ) sin(ϕ1+ ϕ)
− eB_{2c} sin 2ϕ
′
1(δR′− δx′1cot ϕ′1sin ϕ′)2
sin(ϕ′
1 − ϕ′) sin(ϕ′1+ ϕ′)

− eB_{c} (cot ϕ1+ cot ϕ′1)(δx1)2. (A38)

After integration over δR, δR′_{, δx}

1, performed in the Gaussian integration, we are left with

three spatial integration variables ϕ, ϕ′_{, y}

1, and the energy variable. As mentioned above,

the latter gives the temporal δ-funtion,

δ(t01+ t12− t21′ − t_{1}′_{0}) =

v

2δ(Rϕ + R

′_{ϕ}′_{) ,} _{(A39)}

which also lifts the integration over ϕ′_{. Let us take the limit ω}

q ≪ ωin, and neglect the

difference between R and R′ _{and between ϕ}

1 and ϕ′1. Choosing ϕ1as the integration variable

instead of y1, we obtain M(q) ∝ π/2 Z 0 R cos ϕ1dϕ1 ϕ1 Z −ϕ1 dϕ √ R tan ϕ1 sin 2ϕ1 ×

× e2ipR(ϕ1+sin ϕ1cos ϕ1)−2iqR sin ϕ1−4γRϕ1/v_{×}

× cos2ϕ1cos(ϕin− ϕ) cos(ϕout− ϕ). (A40)

The first integration is simply R cos ϕ1dϕ1 = dy1, the factor √R tan ϕ1/ sin 2ϕ1 comes from

the gaussian integration, and the cosines give the angular dependence of the electron-photon

[cos(ϕin,out− ϕ)] and electron-phonon (cos ϕ1) matrix elements. Integration over ϕ gives M(q) ∝ π/2 Z 0 R3/2dϕ1psin ϕ1cos3ϕ1×

× e2ipR(ϕ1+sin ϕ1cos ϕ1)−2iqR sin ϕ1−4γRϕ1/v_{×}

× cos(ϕ_{(sin ϕ}in− ϕout)

1)/ϕ1

+ cos ϕ1cos(ϕin+ ϕout)

.

(A41)

Taking advantage of the limit γR/v ≫ 1, we can focus on short arcs, so that ϕ1 ≪ 1 and

|2p−q| ≪ p. Thus, we expand the exponent to ϕ3

1, while in the prefactor we keep the leading

term at ϕ1 → 0. In the experiment described in the paper, the excitation and detection are

unpolarized, so we simply omit the the expression in the square brackets, which describes the polarization dependence. Denoting Rϕ1 = z, we arrive at

M(q) ∝

∞

Z

0

dz√z e−[i(q−2p)+2γ/v]z−i[p/(12R2)]z3, (A42)

which is Eq. (1) of the main text. The integral is calculated using the relations33,39

1 2π3/2 ∞ Z 0 dt √ t cos xt + t 3 12+ π 4 = Ai2(x), (A43) 1 2π3/2 ∞ Z 0 dt √ t sin xt + t 3 12+ π 4

= Ai(x) Bi(x). (A44)

1 _{A.K. Geim, and K.S. Novoselov, Nature Mat. 6, 183, (2007)}

2 _{K.S. Novoselov, D. Jiang, F. Schedin, T.J. Booth, V.V. Khotkevich, S.V. Morozov, and}

A.K. Geim, PNAS 102, 10451, (2005).

3 _{C. Berger, Z. Song, Z. Li, X. Li, A.Y. Ogbazghi, R. Feng, Z. Dai, A.N. Marchenko, E.H. Conrad,}

P.N. First, and W.A. de Heer, J. Phys. Chem. 108, 19912, (2004).

4 _{P.N. Sutter, J.I. Flege, and E.A. Sutter, Nature Mat. 7, 406, (2008).}

5 _{A.C. Ferrari, J.C. Meyer, V. Scardaci, C. Casiraghi, M. Lazzeri, F. Mauri, S. Piscanec, D. Jiang,}

K.S. Novoselov, S. Roth, and A.K. Geim, Phys. Rev. Lett. 97, 187401, (2006).

6 _{D. Graf, F. Molitor, K. Ensslin, C. Stampfer, A. Jungen, C. Hierold, and L. Wirtz, NanoLett.}

7, 238, (2007).

7 _{C. Faugeras, A. Nerri`ere, M. Potemski, A. Mahmood, E. Dujardin, C. Berger, and W.A. de}

Heer, Appl. Phys. Lett. 92, 011914, (2008).

8 _{A.V. Baranov, A.N. Bekhterev, Y.S. Bobovich, and V.I. Petrov, Opt. Spektrosk. 62, 1036,}

(1987).

9 _{C. Thomsen, and S. Reich, Phys. Rev. Lett 85, 5214, (2000).}

10 _{J. K¨}_{urti, V. Z´}_{olyomi, A. Gr¨}_{uneis, and H. Kuzmany, Phys. Rev. B 65, 165433, (2002).}
11 _{D.M. Basko, Phys. Rev. B 76, 081405(R), (2007).}

12 _{R. Saito, A. Jorio, A.G. Souza Filho, G. Dresselhaus, M.S. Dresselhaus, and M.A. Pimenta,}

Phys. Rev. Lett. 88, 027401, (2002).

13 _{D.L. Mafra, G. Samsonidze, L.M. Malard, D.C. Elias, J.C. Brant, F. Plentz, E.S. Alves, and}

M.A. Pimenta, Phys. Rev. B 76, 233407, (2009).

14 _{J. Hass, F. Varchon, J.E. Millan-Otoya, M. Sprinkle, N. Sharma, W.A. de Heer, , P.N. First,}

L. Magaud, and E.H. Conrad, Phys. Rev. Lett. 100, 125504, (2008).

15 _{C. Berger, Z. Song, X. Li, X. Wu, N. Brown, C. Naud, D. Mayou, T. Li, J. Hass,}

A.N. Marchenkov, E.H. Conrad, P.N. First, and W.A. de Heer, Science 312, 1191, (2006).

16 _{M.L. Sadowski, G. Martinez, M. Potemski, C. Berger, and W.A. de Heer, Phys. Rev. Lett. 97,}

266405, (2006).

17 _{D.L. Miller, K.E. Kubista, G.M. Rutter, M. Ruan, W.A. de Heer, P.N. First, and J.A. Stroscio,}

Science 324, 924, (2009).

18 _{C. Faugeras, M. Amado, P. Kossacki, M. Orlita, M. Sprinkle, C. Berger, W.A. de Heer, and}

M. Potemski, Phys. Rev. Lett. 103, 186803, (2009).

19 _{M. Orlita, C. Faugeras, P. Plochocka, P. Neugebauer, G. Martinez, D.K. Maude, A.-L Barra,}

M. Sprinkle, C. Berger, W.A. de Heer, and M. Potemski, Phys. Rev. Lett. 101, 267601, (2008).

20 _{Z. Ni, Y. Wang, T. Yu, Y. You, and Z. Shen, Phys. Rev. B 77, 235403, (2008).}

21 _{P. Poncharal, A. Ayari, T. Michel, and J.-L Sauvajol, Phys. Rev. B 78, 113407, (2008).}

22 _{J.A. Robinson, C.P. Puls, N.E. Staley, J.P. Stitt, M.A. Fanton, K.V. Emtsev, T. Seyller, and}

Y. Liu, Nano Lett. 9, 964, (2009).

23 _{A. Das, S. Pisana, B. Chakraborty, S. Piscanec, S.K. Saha, U.V. Waghmare, K.S. Novoselov,}

H.R. Krishnamurthy, A.K. Geim, A.C. Ferrari, and A.K. Sood, Nature Nanotech. 3, 210, (2008).

24 _{A. Das, B. Chakraborty, S. Piscanec, S. Pisana, A.K. Sood, and A.C. Ferrari, Phys. Rev. B 79,}

155417, (2009).

25 _{S. Pisana, M. Lazzeri, C. Casiraghi, K.S. Novoselov, A.K. Geim, A.C. Ferrari, and F. Mauri,}

Nature Mat. 6, 198, (2007).

26 _{J. Yan, Y. Zhang, P. Kim, and A. Pinczuk, Phys. Rev. Lett. 98, 166802, (2007).}
27 _{T. Ando, J. Phys. Soc.Jpn. 76, 024712, (2007).}

28 _{M.O. Goerbig, J.-N Fuchs, K. Kechedzhi, and V.I. Falko, Phys. Rev. Lett. 99, 087401, (2007).}
29 _{D.M. Basko, Phys. Rev. B 78, 125418, (2008).}

30 _{T.A. Sedrakyan, E.G. Mishchenko, and M.E. Raikh, Phys. Rev. Lett. 99, 036401, (2007).}
31 _{D.M. Basko, Phys. Rev. B 79, 205428, (2009).}

32 _{P. Carmier and D. Ullmo, Phys. Rev. B 77, 245413, (2008).}

33 _{O. Vall´ee and M. Soares, Airy Functions and Applications to Physics (World Scientific, }

Hack-ensack, 2004).

34 _{In fact, the assumption of the constant phonon density of states is not necessary, since one}

can use the phonon dispersion in the vicinity of the K point which has been recently measured by inelastic x-ray scattering [A. Gr¨uneis, J. Serrano, A. Bosak, M. Lazzeri, S.L. Molodtsov, L. Wirtz, C. Attaccalite, M. Krisch, A. Rubio, F. Mauri, and T. Pichler, Phys. Rev. B 80, 085423, (2009)]. The theoretical curves in Fig. 2 were produced using this experimental disper-sion. However, calculations with a constant phonon density of states lead to an almost similar result (within a few percent).

35 _{Actually, the contribution to γ from electron-electron collisions does acquire a B-dependent}

correction due to the curvature of the electronic trajectories.30 _{However, when the sample is}

not strongly doped, it is reasonable to assume that the main source of electronic scattering is the emission of phonons. The corresponding rate depends on the magnetic field through the electronic density of states. The latter developes oscillations whose amplitude is exponentially small for the non-quantizing field, and the effect analyzed in the paper is indeed the dominant one. For quantizing magnetic fields, the electronic density of states is dominated by Landau levels, which should then be taken into account.

36 _{D.M. Basko, S. Piscanec, and A.C. Ferrari, Phys. Rev. B 80, 165413, (2009).}
37 _{C. Casiraghi, Phys. Rev. B 80, 233407 (2009).}

38 _{P. Plochocka, C. Faugeras, M. Orlita, M.L. Sadowski, G. Martinez, M. Potemski, M.O. Goerbig,}

J.-N Fuchs, C. Berger, and W.A. de Heer, Phys. Rev. Lett. 100, 087401, (2008).

39 _{W.H. Reid, Zeitschrift f¨}_{ur Angewandte Mathematik und Physik 46, 159, (1995).}